Abstract

High strength wires, which have a poor notch sensitivity perfor-mance, are currently been used on many offshore applications where high stresses without yielding are demanded. To assess these wires notch sensitivity, an integrated approach was implemented. An experimental program was conducted, through the realization of fatigue tests to obtain the fatigue limit for notched and notched free specimens to assess the fatigue stress concentration factor. A numerical approach using Finite Element Method, and an analyti-cal model, available in technianalyti-cal literature, were used to assess the stress concentration factor. With both results, the notch sensitivity could be obtained.

Keywords

Fatigue, notch sensitivity, staircase method.

## Assessing the Notch Sensitivity of High Strength Wires

1 INTRODUCTION

The notch sensitivity (q) is a very important design parameter, since its estimation directly influences
the design against fatigue failure of mechanical parts. Also notch sensitivity is associated with many
other mechanical design concepts such as: stress concentration factor (SCF) or *K*t, fatigue *SCF *or *K*f

and short cracks propagation. Indeed, the *SCF* is a well-known parameter used in mechanics of solids
to estimate the stress amplification caused by a mechanical part discontinuity, like a notch. Its
esti-mation depends entirely on the loading type and the geometry of the discontinuity. It is also
well-known that for variable load the stress amplification, for ductile materials, is usually overestimated by

*K*t. To reduce the conservatism in the design of mechanical parts that are subjected to variable

load-ing, the fatigue *SCF *is used. This variable is also a function of notch sensitivity factor (q) that takes

Carlos Filipe Cardoso Bandeira a Paulo Pedro Kenedi a,*

Luis Felipe Guimarães de Souza a

a_{ PPEMM - Programa de Pós-Graduação }
em Engenharia Mecânica e Tecnologia de
Materiais, CEFET/RJ - Av. Maracanã,
229 - Maracanã - RJ - CEP 20271-110 –
Brazil

fillypebandeira@hotmail.com paulo.kenedi@cefet-rj.br luis.felipe@cefet-rj.br

* Corresponding Author

http://dx.doi.org/10.1590/1679-78253728

into account, for notches, both: notch radius (r) and material ultimate strength (Sut), recognizing that

material influences on the stress amplification near notch discontinuity.

Research has been done in this area by Castro and Meggiolaro (2013), which associated the
notch sensitivity with the relatively fast generation of tiny non-propagating cracks at notch root.
According to the authors it indicates that the crack initiation is controlled by the stresses acting at
notch tip and the fatigue crack growth behavior of short cracks emanating from notch root could be
affected by the generated stress gradients. So, a crack could start at a notch tip and then stop after
a short growth, due to the decreasing of the driving force in spite of its growing size. Thus, *q* should
depend not only on the notch tip radius but also on the notch depth. Castro *et al. *(2014) addresses
semi-empirical *q* factors that consider the notch tip stress gradient influencing on the fatigue
behav-ior of short cracks. According to the authors, properly calculation of *q* values can be done from its
fatigue limit (Se), and crack propagation threshold (ΔKth), considering all the notch geometry and

loading characteristics, without the need of any adjustable parameter.

Hu *et al*. (2012) made a review of various concepts that are related to *q *as fracture process
zone, damage process zone and theory of critical distance (TCD), suggesting an exponent *m *to
es-timate *q*. The results indicate that there is an optimal *m* value for each material. Also, Arola and
Williams (2002) evaluated the apparent *K*t of surface texture on the fatigue life of high-strength

low-alloy steels (HSLAS). It was found that the fatigue life of the used *HSLAS *was
surface-texture-dependent, with the fatigue strength decreasing with the increase of the surface roughness.

Chapetti and Gerrero (2013) proposed the integration of fracture mechanics concepts to account
for both: the fatigue notch sensitivity and the notch size effect. In fact, for components tested under
cyclic loading containing notches or holes of a given *K*t, with their fatigue strengths measured, the

smaller are the notch or hole sizes, smaller is the decrement of *K*f value.

In this article, an integrated approach was implemented to estimate the notch sensitivity of
high strength wires (HSW). To accomplish it, *K*f was obtained from experimental results of notched

and notched free specimens. The estimation of *K*t was implemented through the use of finite

ele-ment commercial software, double-checked by an analytic approach as in Young (1989). Thus, the
estimation of *q *was obtained through the utilization of classical relationships between *K*t and *K*f.

2 EXPERIMENTAL APPROACHES

The experimental approaches were divided in: material characterization, fatigue apparatus and fatigue procedure. The material characterization was divided in chemical analysis, tensile tests, optical mi-croscopy, hardness and roughness tests. The fatigue apparatus describes the specimen dimensions, servo-hydraulic machine setup and test accessories. The fatigue procedure explains the staircase meth-od used to determine the fatigue limits. The material characterization is addressed in sequence.

2.1 Material Characterization

properties, such as: Yield Strength (Sy); Ultimate Strength (Sut) and Elongation (EL*)*. For tensile

tests, three specimens of 200 mm length were used with 50 mm gage length for elongation
meas-urements. It can be seen from Tables 1 and 2 that high values of *S*y and *S*ut are consistent with high

strength steels (HSS) and compatible with a SAE 1065 steel material.

Chemical composition in weight

element C Si Mn P S Cr Mo Ni Al

(%) 0.64 0.22 0.74 0.019 0.007 0.037 0.009 0.023 0.028

**Table 1**: Chemical analysis results.

Specimen S (MPa) S (MPa) EL (%)

1 1150 1260 15.3

2 1180 1270 15.0

3 1150 1250 14.6

average 1160 1260 14.9

**Table 2**: Tensile tests results.

The Young modulus and Poison ratio were estimated, respectively, as *E* = 200 GPa and _{ν} =
0.29. Also, it is important to observe that a high *S*ut is directly related to high fatigue resistance

(Sf).

To implement the hardness tests an Instron Wolpert machine was used with a Rockwell C in-denter. To obtain the surface roughness it was used a Tesa-Rugosurf 10 equipment. Tables 3 and 4 show the hardness and the roughness results, respectively.

Test HRC

1 34.8

2 36.0

3 35.5

**average ** **35.4 **

**Table 3**: Hardness results.

Measurement Ra longitudinal Ra transversal

1 0.22 0.58

2 0.14 0.65

3 0.22 0.45

**average ** **0.19 ** **0.56 **

**Table 4**: Roughness results.

(a) (b)

**Figure 1**: Microstructural aspect observed by optical microscopy. (a) Transversal and (b) longitudinal
cross sections. Etching: nital 2%. Magnification: 1000 X. Bandeira *et al. *(2014).

It can be observed that the microstructure is composed of elongated grains, in the rolling di-rection, of ferrite and pearlite. The volumetric fraction of pearlite is consistent with an eutectoid carbon steel composition. It can be also observed fine elongated white areas between pearlite grains which correspond to the primary ferrite. Such microstructural aspect suggests a severe cold working, compatible with the last rolling pass that could be applied under the critical tempera-ture. Such procedure is in line with materials aiming to attain high yield strength and ultimate tensile strength levels. The fatigue apparatus is addressed in sequence.

2.2 Fatigue Apparatus

To experimentally assess *K*f value, it was necessary to obtain the notched and notched free

speci-mens fatigue limits. To accomplish this objective notches and notched free specispeci-mens were tested in a servo-hydraulic test machine, equipped with a four points bending fixture.

The specimens were submitted to different loading levels, maintaining the same loading ratio *R*

= σmin / σmax. All specimens were manufactured in house by cutting 200 mm length bars.

Concern-ing the specimen’s surface finishConcern-ing, they were far from highly polished; indeed all surface finishConcern-ing was maintained as received, with arithmetic average of absolute values of roughness (Ra) shown in

Table 4. In this way, it was considered that the fatigue curves were related to real parts rather than the usual high polished specimens. Fig. 2 shows both specimens types.

(a) (b)

The dimensions were identical for both specimens’ types, notched and notched free, unless by a 0.4 mm shallow notch for the notched specimens generated (at transversal direction) by a broaching process in half its longitudinal length. Figure 3 shows the servo-hydraulic test machine used to im-plement the experimental fatigue tests, where Fig. 3.a shows the servo-hydraulic test machine gen-eral view and Fig. 3.b shows a specimen positioned on the inferior part of the four points bending fixture.

(a) (b)

**Figure 3**: Servo-hydraulic test machine: (a) general view and (b) four points
bending fixture (only the bottom part is shown).

Fig. 4 shows the four points bending fixture schematic drawing that is used to show some im-portant geometric and loading characteristics.

**Figure 4**: The four points bending fixture schematic drawing.

The distances between rollers were defined in function of the specimen length. The bending moment is considered uniform between the upper rollers. The experimental tests were conducted using pulsating loads, to guarantee the upper rollers contact with specimen during the tests. The fatigue loading levels were defined as a ratio between the specimen maximum stress (σmax) and the

The maximum force (Fmax) applied by the test machine was calculated as in Crandall *et al*.

(1978):

F _{a ∙ c}2 ∙ I (1)

Where, *I* is the specimen second moment of area, *a* is the distance between lower and upper
rollers (see Fig.4) and *c* is the specimen semi-height (note that for notched specimen, the notch
depth is deducted).

The four pointsbending apparatus was used, as shown schematically in Fig.4, to apply the
pul-sating load. The ratio was maintained at *R* = 0.1. As the pulsating sine load has nonzero mean
stress it was necessary to transform both, mean stress (σm) and alternating stress (σa), on

equiva-lent alternating stress (_{σ}a_eq), as in Budynas and Nisbett (2014) and Castro and Meggiolaro (2016):

_ _{ or }_

(2)

It is also possible to rewrite equation 2.b to be a function of *σ*a_eq:

σ 2 _

1 1 _ (3)

The fatigue procedure is addressed in sequence.

2.3 Fatigue Procedure

One of the main objectives of this article is focused in obtaining, with maximum possible accuracy,
fatigue limits of both notched and notched free *HSS *specimens. To accomplish this objective the
staircase method was used, as in Dixon (1965) and Dixon (1948). This method uses a simple idea: a
specimen is submitted to a certain stress level, after a certain number of cycles if this specimen
breaks, the next specimen has the stress level decreased by a pre-defined stress decrement. However,
if the specimen doesn’t break, then the stress level is increased by a pre-defined stress increment.
This process continues until all specimens are used or reaches a significant number of specimens
that are statistically representative according to Dixon and Mood (1948). The staircase method
flowchart is presented in Fig. 5. This simple method can produce a much better estimative of the
notched and notched free specimen fatigue limits than the traditional Wohler approach.

Where *C*1 is a positive constant smaller than one that multiplies *S*ut to estimate the first

maxi-mum stress σmax1, *C*2 is a positive constant bigger than one that divides the constant *C*1 to generate

the fraction of *S*ut called stress increment. *s* is the increment or the decrement of stress and *n* is the

number of specimens utilized. *i* is a counter that varies from 1 to n+1. is the *i*th term of
max-imum stress applied to specimen. CPi is an output variable that has two values: *B* or *NB*, which

means that a specimen has broken or has not broken.

**Figure 5**: Staircase method flowchart – specimen test sequence. Pollack *et al*. (2006)

3 NUMERICAL APPROACH

It is well known that the *SCF *produced by a given notch depends on the mode of loading and on
the notch geometry. There are many ways to estimate it: by theory of elasticity, as in Timoshenko
and Goodier (1951); by experimental measurements as in Pilkey and Pilkey (2008); using, for
ex-ample, photoelasticity method, as in Dally and Riley (1991), or by using a numerical method like
finite element method, as in Fish (2007). In this section a numerical approach, using finite element
method, is used to estimate the stress concentration factor of the shallow notch.

3.1 Numerical Model

In this article it was used the commercial software ANSYS WORKBENCH v14.0 to evaluate *SCF *

produced by a shallow notch broached on *HSS *specimen. For numerical model purposes the
speci-men material was considered isotropic and linear elastic. The mesh was generated with hexahedrons
elements PLANE 186 with plane stress option, with one node at each vertex, as shown in Fig. 6.a.
The finite element model was created in 2-D dimension (in the X-Y plane) to reduce the
computa-tional effort, as shown in Fig. 6.b.

The 2D model with plane stress option was considered based on E399 ASTM standard (2009).
In item 7.1.3 of this standard, the minimum specimen width to develop plane strain condition is
related to the material Sy/E ratio. Using the *HSS *material properties, this ratio was calculated as

suppose that the state of stress is much closer, even at half specimen width, to plane stress than to plane strain condition.

(a) (b)

**Figure 6**: Finite element model: (a) element PLANE 186 and (b) 2-D geometry.

Due to the notch depth is much smaller than the specimen height, in fact it is a shallow notch, and to ensure good elements aspect ratio, mainly around the notch, a refined region around it was provided as shown in Fig. 7.a. Figure 7.b shows a photo of the real notch machined by a manual broaching machine.

(a) (b)

**Figure 7**: (a) Specimen mesh details (*δ* = 0.075 mm) and (b) optical microscopy photo of the notch.

**Figure 8**: Mesh convergence study.

The mesh refinement of *δ* = 0.075 mm was selected for this analysis because the notch
bounda-ry can be described with a reasonable accuracy. Both, experimental and numerical results are
pre-sented at the next section.

4 RESULTS

The results are divided in two parts: experimental and numerical. At experimental part, the fatigue
limit results obtained from the experimental tests are shown and, at numerical part, the *SCF* result
obtained from the finite element method is shown.

4.1 Experimental Results

Fig.9 shows a representation of the test sequence, for both notched and notched free specimens,
applying the staircase method, as in Pollack *et al*. (2006), which algorithm can be seen in Fig. 5.

(a) (b)

Note that all stresses are divided by *S*ut, generating a ratio (*σ*a_eq / *S*ut)·100, which varies from 0

to 100%. Fig.10 presents all fatigue results, with common points that were obtained by usual fa-tigue approach and up-and-down points by using staircase method. The common points are repre-sented by black squares and the up-and-down points are reprerepre-sented by blue circles. Note that an arrow represent that specimen didn’t fail, for all figures. There is one arrow per specimen, unless in Fig. 10.b, where the not broken specimens were so near each other, that just one arrow was used.

(a) (b)

**Figure 10**: Fatigue results: both common points and up-and-down points for
(a) notched free, (b) notched specimens.

The fatigue results which are graphically shown in Fig. 10, correspond to actual fatigue results
values that are shown at Appendix, in Tables 6 and 7. Also in Fig. 14, at the same Appendix, the
staircase method flowchart explains, in a graphical way, the two *S*e estimation, which are

represent-ed by blue lines in Fig. 10. In Figs. 11.a and 11.b show a detailrepresent-ed view of up-and down points.

(a) (b)

The fatigue limit results shown on Table 5 were obtained through the utilization of staircase
method flowchart – estimation of *S*e range, shown in Fig. 14 at Appendix. The experimental fatigue

results are available at Tables 6 and 7, also at Appendix, or graphically in Fig. 10.

Specimen μ σ Fatigue Limit (%)

Common points

notched free 35.5 4.5%_{4.5%} 33.9 ≤ ⁄ ∙ 100 ≤ 37.1

notched 15.5 4.5%

4.5% 14.8 ≤ ⁄ ∙ 100 ≤ 16.2

Up-and-down points

notched free 32.7 1.1%_{1.0%} 32.3 ≤ ⁄ ∙ 100 ≤ 33.0

notched 12.7 1.1%_{1.0%} 12.6 ≤ ⁄ ∙ 100 ≤ 12.8

Note: *μ*and *σ* were maintained from the notation adopted in Pollack *et al*. (2006).

**Table 5**: Fatigue limits, mean *μ* and the standard deviation *σ*.

The mean and the standard deviation of fatigue limit, respectively, *μ* and *σ*, of Table 5 were
as-sessed for two cases: if the failures were the majority event, the lower stress level of survival
occur-rence was estimated or if the survivals were the majority event, the lower stress level of failure
oc-currence was estimated. Note in Table 5 that fatigue limit for both notched and notched free
spec-imens were estimated with less dispersion when it was used the up-and-down approach, based in the
staircase method when compared with the common points, obtained with usual approach.

The numerical results were assessed in sequence.

4.2 Numerical Results

To calculate the *SCF*, the specimen model was loaded in pure bending, to simulate the four points
bending test. The bending moment value was imposed to generate a unity normal stress on
longitu-dinal fiber at the same height of the notch root but far from it. Using this approach, the maximum
stress value at the notch root turns out to be exactly the value of the *SCF*. Fig. 12.a shows the
finite element results in a usual representation and in Fig.12.b it was used a path approach, at the
same height of the notch root, to explicitly show the stress concentration distribution.

As expected, the stresses form a high gradient curve in the neighborhood of the shallow notch
root. The ratio between maximum stresses at notch root and nominal stresses at a region far from
notch, was used to estimate *K*t:

K _{σ} σ _ 2.84_{1} 2.84 (4)

Note that using the analytical approach shown at Appendix the *K*t was estimated as 2.79,

which is quite close to the finite element estimative of 2.84. So, the value was estimated inside the following range: 2.79 2.84.

(a)

(b)

**Figure 12**:Finite element longitudinal stresses (*x*-axis): (a) usual presentation
and (b) path approach (only left half is shown).

5 DISCUSION

In this section the results obtained by experimental and numerical approaches are used to estimate
the *HSW *notch sensitivity factor.

The fatigue limit range for each specimen condition can be obtained from Table 5: 32.3

≤ _⁄ ∙ 100 ≤ 33.0 and 12.6 ≤ ⁄ ∙ 100 ≤ 12.8. The fatigue stress

con-centration factor can be stated, as Budynas and Nisbett (2014):

K _⁄_{⁄} (5)

So the fatigue stress concentration factor *K*f can be estimated, within the following range: 2.56
2.58. In sequence, the notch sensitivity can be estimated through the utilization of a classic
Peterson’s equation, as Budynas and Nisbett (2014):

q _{K}K 1_{1} (6)

Finally, applying the ranges calculated, respectively *SCF* and fatigue *SCF *ranges in equation
(06), the range within the notch sensitivity can be estimated as: 0.86 0.87.

effec-tive, manly due the use of the staircase method in the assessment of fatigue limits of the notched and the notched free specimens. On the other hand, the notch sensitivity range revealed to be high, indicating a probable brittle behavior, which is compatible to high strength materials. In fact, alt-hough the high ultimate strength is a desirable mechanical property to increase the fatigue re-sistance, the high notch sensitivity can induce deleterious effects to mechanical structures submitted to fatigue loading.

6 CONCLUSIONS

An integrated approach was used to assess the notch sensitivity of *HSW*. Material characterization
was obtained through the implementation of chemical analysis, tension tests, hardness tests,
rough-ness tests and optical microscopy of the *HSW*. Fatigue tests were accomplished with two types of
wire specimens, the notched and the notched free, resulting in very distinct fatigue limits, which
were used to estimate the fatigue *SCF*. Finite element method and analytical approaches were used
to estimate the *SCF* with good matches between them. Finally, the notch sensitivity factor was
obtained through the utilization of a well know Peterson’s equation.

In fact the utilization of the experimental/numerical integrated approach for this research was
revealed quite promising in generating an estimative of *HSW *notch sensitivity value. In particular,
the utilization of staircase method at experimental approach, really improves the fatigue limit
esti-mation, which taking into account the natural tendency of fatigue results dispersion, contributed, in
a very significant way, to obtain such a reasonable estimative of notch sensitivity.

References

Arola, D., Williams C.R. (2002). Estimating the fatigue stress concentration factor of machined surfaces. Int. Journal of Fatigue, 24: 923-930.

Bandeira, C.F.C., Kenedi. P.P. and Souza, L.F.G. (2014). Analysis of Notch Sensitivity of High Strength Wires. VIII Congresso Nacional de Engenharia Mecânica – CONEM 2014, Uberlândia, Brazil.

Budynas, R. G. and Nisbett, J. K. (2014). Shigley's Mechanical Engineering Design. 10th Edition. McGraw Hill Education.

Castro, J.T.P. and Meggiolaro, M.A. (2016). Fatigue Design Techniques under Real Service Loads – Volume I – High-Cycle Fatigue, Amazon Books

Castro, J.T.P., Landim, R.V., Leite, J.C.C., Meggiolaro, M.A. (2014). Prediction of notch sensitivity effects in fa-tigue and in environmentally assisted cracking. Fafa-tigue Fract Engng Mater Struct, 38:161–179, doi: 10.1111/ffe.12156.

Castro, J.T.P. and Meggiolaro, M.A. (2013). Is notch sensitivity a stress analysis problem? Frattura ed Integrità Strutturale, 25: 79-86, DOI: 10.3221/IGF-ESIS 25.12.

Chapetti, M.D., Guerrero, A.O. (2013). Estimation of notch sensitivity and size effect on fatigue resistance. Procedia Engineering, 66:323-333.

Crandall, S.H., Dahl, N.C., Lardner, T.J. (1978). An Introduction to the Mechanics of Solids. Second Edition with SI units, McGraw Hill International Editions.

Dixon, W.J., Mood, A.M. (1948). A method for obtaining and analysing sensitivity data. J. Am. Stat. Assoc. 43: 109–126.

E399_09 ASTM standard (2009). Linear Elastic Plane Strain Fracture Toughness KIC of Metallic Materials. Fish, J. (2007). A First Course in Finite Elements. Wiley. ISBN-10: 0470035803.

Hu, X. A., Yang, X. G., Wang, J. K., Shi, D. Q., Huang, J. (2012). A simple method to analyze the notch sensitivi-ty of specimens in fatigue tests. Fatigue Fract Engng Mater Struct, 36:1009–1016, doi: 10.1111/ffe.12053.

Pilkey W.D. and Pilkey, D.F. (2008). Peterson's Stress Concentration Factors. 3rd Edition, Wiley.

Pollak, R., Palazotto, A., Nicholas, T. (2006). A simulation-based investigation of the staircasemethod for fatigue strength testing. Mechanics of Materials, 38:1170-1181.

Thimoshenko, S. and Goodier, S.N. (1951). Theory of Elasticity. McGraw-Hill.

Yang, Z., Kim, Kim, C.B., Cho,C., Beom,H.G. (2008).The concentration of stress and strain in finite thickness elas-tic plate containing a circular hole. International Journal of Solids and Structures, 45:713-731.

Young, W.C., (1989) Roark’s Formulas for Stress and Strain. Sixth Edition with SI units, McGraw Hill International Editions.

APPENDIX

A.1. Expressions for SCFs:

Fig. 13 shows the geometry of the notches used by analytic approach:

(a) (b)

**Figure 13**: *SCF*s for rectangular cross-section beam submitted to pure moment:
(a) U notch and (b) V notch. Young (1989).

The estimative of *SCF*s shown in Fig.13.a is, Young (1989):

k K for 0.5 ⁄ 4.0

where,

0.721 2.394 ∙ ⁄ 0.127 ∙ ⁄ 0.426 8.827 ∙ ⁄ 1.518 ∙ ⁄

2.161 10.968 ∙ ⁄ 2.455 ∙ ⁄ 1.456 4.535 ∙ ⁄ 1.064 ∙ ⁄

K _ k

The estimative of *SCF*s shown in Fig.13.b is, Young (1989):

According to Young (1989) the *SCF*s of a V–notch is estimated as the smaller value between

*K*t_U and *K*t_V..For this particular case where *h* = 0.4 mm, *r* = 0.3 mm, *h*/*r* = 1.33 mm, *D* = 6

mm and *θ* = 45º, the results are *K*t_U = 2.79 and *K*t_V. = 2.88, which results in an estimative of *K*t

= 2.79.

A.2. Flowchart:

Fig. 14 shows a staircase method flowchart to estimate of *S*e range, as shown in Fig.10:

**Figure 14**: Staircase method flowchart – Estimation of *S*e range. Pollack *et al*. (2006).

Where *A*, *B* and *C* are constants defined in the flowchart, *i*_max is number of specimens that
have survived if the failures was the majority event (FME), *S*0 is the lower stress level of survival

occurrence and *m*i corresponds to the number of specimens which have survived at each stress level
**or ***i*_max is number of specimens that have failed if the survival was the majority event (SME), *S*0

is the lower stress level of failure occurrence and *m*i corresponds to the number of specimens which

have failed at each stress level. *S*e is the fatigue limit; *μ* and *σ* are, respectively, the fatigue limit

A.3. Tables:

Several tests were performed with two types of specimen. Tables 6 and 7 summarize the results.

∙ 100 (%) _ _{∙ 100}_{ (%)}

number of cycles common set 0 up-and-down set 0 up-and-down set 1

50 31 1866774 1012461 1017371

52 32.8 - 174463 185197

54 34.6 - 1021397 166963

56 36.4 - 205270 -

60 40.3 138934 - -

70 51.2 75026 - -

80 64.3 44790 - -

90 80.2 36380 - -

**Table 6**: Fatigue test results – notched free specimens.

∙ 100 (%) _ _{∙ 100}_{ (%) }

number of cycles common set 0 common set 1 common set 2 up-and-down set 0 up-and-down set 1 up-and-down set 2

18 9 - - - 1011280 - -

21.5 11 1163500 - - 1093159 1001769 -

24.9 13 - - - 1042841 344703 788188

28.2 15 - - - 178635 - -

35.7 20 105162 76117 90535 - - -

46.4 28 47501 32698 28350 - - -

55.6 36 24117 20234 20420 - -

66.3 47 16000 13501 12040 - - -

91 82 6141 - - - - -

**Table 7**: Fatigue test results – notched specimens.